Chem. Mater. 2010, 22, 2175–2177 2175 DOI:10.1021/cm1004032
Selective Nucleation and Growth of Cu and Ni Core/Shell Nanoparticles Kyler J. Carroll,† Scott Calvin,‡ Thomas F. Ekiert,§ Karl M. Unruh,§ and Everett E. Carpenter*,† † Department of Chemistry, Virginia Commonwealth University, Richmond, Virginia 23284, ‡Department of Physics, Sarah Lawrence College, 1 Mead Way, Bronxville, New York 10708, and §Department of Physics and Astronomy, University of Delaware, Newark, Delaware 19716
Received February 8, 2010 Revised Manuscript Received March 3, 2010
The physical and chemical properties of metallic core/ shell nanoparticles (CSNPs) can differ in significant ways from the corresponding bulk materials, as well as chemically homogeneous nanoparticles of the same overall composition.1 These observations have led to great interest in the development of new synthesis strategies that can be used to prepare CSNPs, particularly if they are straightforward to implement and can be applied to potentially useful materials. Motivated by these considerations, we have developed a simple chemical procedure for the preparation of Cu core/Ni shell (Cu/Ni) and Ni core/Cu shell (Ni/Cu) CSNPs based on the well-known polyol method.2 Because of their potentially useful catalytic and magnetic properties, we have focused exclusively on the Cu-Ni system,3 although we believe the general approach described below may be applicable to other important materials systems as well. Various implementations of the polyol method have previously been used to prepare elemental Cu nanoparticles, Ni nanoparticles, and Cu-Ni nanoalloys.4 To the best of our knowledge, however, there has only been one *Corresponding author. E-mail: [email protected]
(1) (a) Cozzoli, P. D.; Pellegrino, T.; Manna, L. Chem. Soc. Rev. 2006, 35, 1195. (b) Salgueiri~no-Macereira, V.; Correa-Duarte, M. A. Adv. Mater. 2007, 19, 4131. (c) Sastry, M.; Swami, A.; Mandal, S.; Selvakannan, P. R. J. Mater. Chem. 2005, 15, 3161. (2) Willard, M. A.; Kurihara, L. K.; Carpenter, E. E.; Calvin, S.; Harris, V. G. Int. Mater. Rev. 2004, 49, 125. (3) (a) Chatterjee, J.; Bettge, M.; Haik, Y.; Jen Chen, C. J. Magn. Magn. Mater. 2005, 293, 303. (b) Kuznetsov, A. A.; Leontiev, V. G.; Brukvin, V. A.; Vorozhtsov, G. N.; Kogan, B. Y.; Shlyakhtin, O. A.; Yunin, A. M.; Tsybin, O. I.; Kuznetsov, O. A. J. Magn. Magn. Mater. 2007, 311, 197. (c) Li, P.; Liu, J.; Nag, N.; Crozier, P. A. J. Catal. 2009, 262, 73. (4) (a) Bonet, F.; Grugeon, S.; Tarascon, J. M. J. Solid State Chem. 2003, 172, 111. (b) Chinnasamy, C. N.; Jeyadevan, B.; Shinoda, K.; Tohji, K.; Narayanasamy, A.; Sato, K.; Hisano, S. In Proceedings of the 49th Annual Conference on Magnetism and Magnetic Materials; Jacksonville, FL, Nov 7-11, 2004; American Institute of Physics: College Park, MD, 2005; Vol. 97, p 10J309. (c) Fievet, F.; Fievet, F. V.; Lagier, J. P.; Dumont, B.; Figlarz, M. J. Mater. Chem. 1993, 3, 627. (d) Park, B. K.; Jeong, S.; Kim, D; Moon, J.; Lim, S.; Kim, J. S. J. Colloid Interface Sci. 2007, 311, 417. (e) Shengming, J.; Liangsheng, Y.; Ying, Z.; Guanzhou, Q.; Cuifeng, W. Mater. Res. Bull. 2006, 41, 2130. (f) Sun, J.; Jing, Y.; Jia, Y.; Tillard, M.; Belin, C. Mater. Lett. 2005, 59, 3933. (g) Zhang, X.; Yin, H.; Cheng, X.; Jiang, Z.; Zhao, X.; Wang, A. Appl. Surf. Sci. 2006, 252, 8067. r 2010 American Chemical Society
previous report in which the polyol method was used to prepare CSNPs consisting of elemental Cu and Ni.4a In that case, Cu/Ni CSNPs were obtained after heating hydrated Cu and Ni nitrates dissolved in ethylene glycol (EG) for 4 h at 196 °C. The formation of a core/shell structure was attributed to the different thermal stabilities of Cu and Ni glycolates formed during the reaction. In particular, the transformation of Cu glycolate to elemental Cu was observed to precede the transformation of Ni glycolate to elemental Ni. The Cu nanoparticles then served as a heterogeneous nucleation site for the deposition of Ni, leading to the formation of a core/shell structure. In this work, a series of experiments were carried out in which hydrated Cu chloride (CuCl2 3 2H2O), hydrated Ni chloride (NiCl2 3 6H2O), and sodium hydroxide (NaOH) were dissolved in EG and rapidly heated to the boiling point of the solution. By exploiting the strong dependence of the boiling temperature of these solutions on the relative quantities of dissolved salt, the associated water of hydration, NaOH, and solvent, two stabilized reaction temperatures could be obtained without the need for active temperature control by simply switching between reflux and distillation conditions. In particular, a solution containing 0.5 g of Cu chloride, 0.5 g of Ni chloride, and 3 g of NaOH dissolved in 25 mL of EG was found to boil at a temperature of about 165 °C, well below the temperature of 196 °C at which the EG itself boiled (pure EG boils at about 197 °C). After removing the water of hydration from the solution, the boiling point was observed to increase to about 175 °C. This 10° difference was sufficient to separate the formation of elemental Cu under reflux conditions from the formation of elemental Ni under distillation conditions. At the reflux temperature of 165 °C, the Cu reaction was complete in less than 30 min, ensuring that elemental Ni (rather than a Cu-Ni alloy) was formed during the highertemperature distillation step of the reaction. As noted earlier, Cu/Ni CSNPs formed because the Cu nanoparticles served as preferential nucleation sites for the deposition of Ni. Although the temperature was the reaction parameter used to separate the formation of elemental Cu and Ni in these experiments, it is worth noting that the presence or absence of water may also play an important role in the actual reaction mechanism. The asymmetry of the reaction conditions that allowed the formation of Cu/Ni CSNPs does not allow the formation of Ni/Cu CSNPs from a mixed metal-salt solution. Nevertheless, a modification of the procedure described above allowed Ni/Cu nanoparticles to be prepared in a two-step process. In the first step, a Ni chloride solution was distilled until Ni nanoparticles were formed. After completion of the reaction (which could also be terminated prior to completion by quenching the solution in an ice bath) a Cu chloride solution was added and
Published on Web 03/18/2010
Chem. Mater., Vol. 22, No. 7, 2010
Carroll et al.
Figure 3. Room-temperature hysteresis loops for the Cu/Ni (blue) and Ni/Cu (red) CSNPs. The magnetization axis has been scaled based on the ICP-OES measured composition to indicate the magnetization per gram of Ni in the sample. Figure 1. TEM images and composition maps from EDX (red and blue corresponding to Cu and Ni, respectively) of typical of (A, B) Cu/Ni and (C, D) Ni/Cu CSNPs. The uncolored coating on the composition maps corresponds to residual organic material.
Figure 2. XRD patterns of elemental Cu, Cu/Ni, Ni/Cu, and elemental Ni. The elemental metals were prepared using the respective metal chlorides (see the Supporting Information).
heated at reflux leading to the formation of Cu shells on the Ni nanoparticles. The composition, structure, and magnetic properties of the Cu/Ni and Ni/Cu CSNPs were characterized by inductively coupled plasma-optical emission spectroscopy (ICPOES), transmission electron microscopy (TEM) with energy dispersive elemental analysis (EDX), powder X-ray diffraction (XRD), X-ray absorption spectroscopy (XAS), and vibrating sample magnetometry (VSM) measurements. These measurements were used to verify the formation of a core/shell structure and established that the core and shell materials were essentially pure elemental Cu and Ni. TEM images of typical Cu/Ni and Ni/Cu CSNPs and the corresponding composition maps of elemental Cu and Ni distributions are shown in Figure 1. These data clearly show the formation of core/shell type structures. The XRD patterns of the Cu/Ni and Ni/Cu CSNPs are shown in Figure 2. The fitted line positions yielded best fit Cu lattice parameters of 0.3609(13) and 0.3609(6) nm for the Cu/Ni and Ni/Cu CSNPs, respectively, with corresponding Ni lattice parameters of 0.3519(4) and 0.3529(15) nm. Within the experimental uncertainties, these values are consistent with the bulk Cu (0.36148 nm) and Ni (0.35232 nm) lattice (5) Villars, P. Pearson’s Handbook of Crystallographic Data for Intermetallic Phases; American Society for Metals: Metals Park, OH, 1989.
parameters,5 indicating that in both cases the core and shell material comprises essentially unalloyed elemental Cu and Ni. In the case of the Ni/Cu CSNPs, we were also able to obtain XAS data for comparison with the XRD data. Analysis of the extended X-ray absorption fine structure (EXAFS) region of these data yielded a Cu lattice parameter of 0.3623(5) nm and a Ni lattice parameter of 0.3534(6) nm.6 In addition, the second and third cumulants of the Cu-Cu and Ni-Ni interatomic distances, corresponding to the variance and asymmetry of those distances, were also consistent with unalloyed elemental Cu and Ni. The corrected room-temperature hysteresis loops of the Cu/Ni and Ni/Cu CSNPs are shown in Figure 3. The saturation magnetization was obtained by extrapolating a fit of the measured high field magnetization versus the inverse of the applied magnetic field to infinite field. This procedure yielded saturation magnetization values of 18.15(3) emu/g and 19.65(3) emu/g of sample(i.e., based on the total sample mass) for the Cu/Ni and Ni/Cu CSNPs. Assuming the presence of only elemental Cu and Ni in these materials and that all the Ni atoms carry the bulk Ni magnetic moment of 54.4 emu/g, the saturation magnetization values result in particle compositions (at %) of Cu64Ni36 for the Cu/Ni CSNPs and Ni38Cu62 for the Ni/Cu CSNPs. The compositions of the core/shell nanoparticles were also directly determined by ICP-OES. These measurements yielded average compositions of Cu59Ni41 and Ni45Cu55. The origin of the somewhat larger ICP-OES Ni concentrations relative to the magnetization based values is currently under investigation but may arise from a small (and undetected) amount of alloying at the core/shell interface resulting in a reduced Ni moment for interface Ni atoms. Alternatively, a reduced Ni moment due to finite size effects could account for this discrepancy.7 In conclusion, we have identified a new and simple procedure for separating the formation of elemental Cu (6) EXAFS lattice parameters are calculated from the mean nearestneighbor distance. Because of thermal and structural disorder, this yields a “lattice constant” that is somewhat larger than that implied by the long-range order that XRD measures. As with XRD, the values for the sample were consistent with those found for bulk standards. (7) (a) Jiao, J.; Seraphin, S.; Wang, X.; Withers, J. C. J. Appl. Phys. 1996, 80, 103. (b) Jeon, Y. T.; Moon, J. Y.; Lee, G. H.; Park, J.; Chang, Y. J. Phys. Chem. B 2005, 110, 1187.
and Ni in a polyol-type reaction. In particular, the formation of Cu/Ni CSNPs from a mixed metal-salt/NaOH/ EG solution was facilitated by manipulating the boiling temperature of the solution. A two step procedure in which Ni nanoparticles were first prepared from a Ni chloride solution followed by the addition of a Cu chloride solution was also used to prepare Ni/Cu CSNPs.
Chem. Mater., Vol. 22, No. 7, 2010
Acknowledgment. This research was partially funded through an out-of-state graduate teaching fellowship supported by Altria Client Services (Philip Morris USA). Supporting Information Available: Experimental procedures and characterization data of the CSNPs (PDF). This material is available free of charge via the Internet at http://pubs.acs.org.